Journal of Polymers

Volume 2013 (2013), Article ID 523941, 6 pages

http://dx.doi.org/10.1155/2013/523941

Research Article

Phototrophic Growth and Accumulation of Poly(3-hydroxybutyrate-co-3-hydroxyvalerate) by Purple Nonsulfur Bacterium Rhodopseudomonas palustris SP5212

M. Mukhopadhyay,¹ A. Patra,² and A. K. Paul³

¹Department of Microbiology, Lady Brabourne College, Kolkata, West Bengal 700 017, India

²Department of Chemistry, University of Calcutta, Kolkata, West Bengal 700 009, India

³Microbiology Laboratory, Department of Botany, University of Calcutta, Kolkata, West Bengal 700 019, India

Received 27 March 2013; Accepted 13 September 2013

Academic Editor: Changwoon Nah

Copyright © 2013 M. Mukhopadhyay et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

The ability of the phototrophic bacterium Rhodopseudomonas palustris SP5212 to produce polyhydroxyalkanoates (PHAs), poly(3-hydroxybutyrate-co-3-hydroxyvalerate) [P(3HB-co-3HV)] in particular was, assessed in acetate medium supplemented with hydroxybutyrate and valerate as cosubstrates. The isolate accumulated the polymer accounting for some 49.06% and 30% of cell dry weight when grown in hydroxybutyrate and valerate, respectively. PHA accumulation as well as 3HV monomer incorporation (30 mol%) was maximum at 0.1% hydroxybutyrate, while valerate at 0.1% and 0.3% was suitable for total polymer accumulation and 3HV monomer incorporation, respectively. Cosupplementation of hydroxybutyrate and valerate in the ratio of 3 : 1 led to the accumulation of PHA accounting for 54% of cell dry weight, which contained more than 50 mol% of 3HV monomer. Moreover, the biphasic cultivation conditions with hydroxybutyrate as cosubstrate have improved the quality as well as quantity of the accumulated copolymer significantly.

1. Introduction

Polyhydroxyalkanoates (PHAs) represent a unique class of environmentally biodegradable polymers of commercial importance. They are synthesized and accumulated as intracellular carbon and energy rich reserve materials by a wide variety of bacteria when grown under conditions of carbon excess and at least one of the nutrients becomes limiting [1, 2]. PHAs serve as a sink for reducing equivalents depending on the organisms and the physiological conditions of the cells. Accumulated PHAs also play a significant role in the survival of the producer microorganisms under conditions of environmental stress such as osmotic pressure, desiccation, and UV-irradiation [3]. Moreover, they have received increased attention as alternatives to conventional hydrocarbon based thermoplastics mainly because of their material properties, biodegradability, and biocompatibility.

The incorporation of 3-hydroxyvalerate (3HV monomer) into the polymer of 3-hydroxybutyrate (3HB) can result in the synthesis of poly(3-hydroxybutyrate-co-3-hydroxyvalerate) [P(3HB-co-3HV)] with improved thermoplastic properties that are more suitable for commercial application [4]. It is, therefore, apparent that the PHA materials can be tailored to specific applications by varying their chemical structure [5], which could be achieved by variation of producing organisms, carbon sources, cosubstrates and cultural conditions.

Altogether, 150 hydroxyalkanoic acids have been identified as constituents of PHAs [6], and these subunits of PHA have been broadly subdivided as short chain length (C3–C5) and medium chain length (C6–C14) monomers. PHAs composed of different molar proportions of these monomers differ markedly in terms of their physicochemical, mechanical, and thermal properties [7].

Quantitative studies on PHA metabolism by phototrophic purple nonsulfur bacteria are restricted only to a few species like Rhodospirillum rubrum [3], Rhodobacter sphaeroides [8–12], and Rhodopseudomonas palustris [13, 14]. R. palustris, the widely known species of purple non sulfur bacteria, accumulate P(3HB) [13, 15] but only to a limited scale. Vincenzini et al. [16] have reported that R. palustris 420l accumulate P(3HB) of nearly 18% of cell dry weight (CDW) when grown in phosphate limiting condition in a biphasic growth mode. The same isolate, in a temperature controlled underwater tubular photobioreactor in outdoor conditions, produces the highest amount of P(3HB) (4.0% of CDW) in summer in comparison to its lowest accumulation (1.1% of CDW) during winter. R. palustris cells when grown diazotrophically with acetate were reported to accumulate 1.1% to 0.3% of CDW of P(3HB), but under nitrogen fixing condition they are known to accumulate 8.8% P(3HB) of CDW after exhaustion of ammonium from the medium. The species along with Blastochloris sulfoviridis accumulate P(3HB) accounting for 1.4–3.6% of CDW in a lighted upflow anaerobic sludge blanket (LUSAB) [17].

Very little was known about the potential incorporation of monomer units other than 3-hydroxybutyrate into the polymer, leading to the formation of various 3-hydroxyalkanoate copolymers by this particular species. R. palustris 1850 and 17001 incorporated 3HV monomer unit in the polymer when grown with valerate, heptanoate, and octanoate. However, strain 1850 was unable to incorporate 3HV when grown with propionate [9]. R. palustris SP5212 isolated in this laboratory has been reported to accumulate P(3HB) accounting for 15.0% of cell dry weight with acetate as substrate and was capable of utilizing C2–C8 alkanoic acids for growth and polymer production [14]. The objective of the present study was to evaluate the synthesis of copolymers of poly(3-hydroxybutyrate-co-3-hydroxyvalerate) by R. palustris SP5212 and to optimize the cultural conditions for such PHA accumulation. A biphasic cultivation method with alkanoic acid as cosubstrate has also been implemented for qualitative and quantitative improvement of the accumulated polymer.

2. Materials and Methods

2.1. Bacterial Strain and Cultural Condition

Rhodopseudomonas palustris SP5212 reported from this laboratory [14] was used throughout this study. The isolate was grown in 15 mL screw cap bottles under microaerobic phototrophic conditions using malate medium (g/L, malic acid, 0.2; K₂HPO₄, 0.9; KH₂PO₄, 0.6; MgCl₂, 0.2; nicotinic acid, 0.005, EDTA, 0.02; NH₄Cl, 1.0; yeast extract, 1.0 (pH 6.8)). The same medium with minor modifications was used for PHA accumulation. Malate was replaced by acetate as the main carbon source, ammonium chloride was omitted to induce nutritional stress, and alkanoic acids were supplemented as the cosubstrate. Experiments were conducted in 300 mL transparent glass stoppard bottles. The medium was inoculated with a freshly grown culture (O.D. 0.5 at 650 nm) at 2.0% (v/v) level and incubated under microaerophilic condition with a continuous illumination (10,000 lux) at C.

For biphasic growth experiments, R. palustris SP5212 was initially grown in malate medium for 4 days, and cells were harvested aseptically, washed thoroughly with sterile 0.9% NaCl, and transferred to a similar 300 mL transparent glass stoppard bottle containing acetate medium. The medium was supplemented with alkanoic acids and incubated under continuous illumination (10,000 lux) at C.

2.2. Determination of Growth

Growth of the organism was determined by measuring the dry weight of the biomass. Cells were harvested by centrifugation at 12,500 ×g in a Hitachi SCR 20B centrifuge, washed thoroughly, transferred to preweighed aluminium cups, and dried to a constant mass at C.

2.3. Analysis of Polyesters

The polymer was extracted from the dried cell mass directly with boiling chloroform [19], concentrated and precipitated with double volume of prechilled diethyl ether, separated by centrifugation (12,000 g for 10 min), and dried under vacuum at room temperature. For purification, the polyester was redissolved in chloroform, filtered and further precipitated with chilled diethyl ether, and dried under reduced pressure. The amount of PHA was quantified gravimetrically and expressed as the percentage of cellular dry weight [18]. Monomer composition of the PHAs was determined by ¹H NMR spectroscopic analysis. The purified polymer, dissolved in analytical grade deuterochloroform (CDCl₃), was subjected to analysis, and the chemical shifts were recorded using a Bruker AMX 300 NMR spectrophotometer with a multinucleate probe head.

3. Results and Discussions

Time course of growth and polymer accumulation by R. palustris SP5212 under phototrophic conditions in the acetate medium supplemented with hydroxybutyric acid (0.1% w/v) as cosubstrate revealed gradual increase in growth and polymer accumulation with the period of incubation. The accumulated polymer attained its maxima after 12 days of incubation (Figure 1(a)) when the PHA content reached 49.06% of cell dry weight (CDW). It was evident that during the early stages of growth there was no incorporation of 3-hydroxyvalerate (3HV) in the polymer but with time the 3HV monomer unit incorporation in the P(3HB-co-3HV) increased up to 37 mol% after 10 days of growth (Figure 1(b)). Similarly, supplementation of valeric acid as cosubstrate also revealed similar pattern of growth and 3HV incorporation in the polymer (Figure 2(a)). At 12 days of growth the accumulated PHA (30% CDW) of R. palustris cells contained nearly 14 mol% of 3HV monomer unit (Figure 2(b)). The present experimental results have clearly established the synthesis of poly(3-hydroxybutyrate-co-3-hydroxyvalerate) [P(3HB-co-3HV)] by R. palustris SP5212 utilizing hydroxybutyrate as well as valerate as cosubstrate and acetate as the principal source of carbon. Most of the earlier studies with R. palustris reported accumulation of only P(3HB) under different cultural conditions [13, 15, 17]. However, accumulation of copolymers containing C4-C5 monomers was reported only when the organism was grown on alkanoic acids [9, 14]. Rhodopseudomonas acidophila accumulated polymer with 91.0 mol% of 3HV when grown with C5 compounds [9]. In contrast, Rhodospirillum rubrum accumulated copolymers of C4, C5, and C6 compounds with higher carbon substances [3].

(a)

(b)

Figure 1: Time course of growth, PHA content (a), and composition (b) of the polyester accumulated by R. palustris SP5212 under phototrophic conditions in acetate medium supplemented with hydroxybutyrate as cosubstrate.

(a)

(b)

Figure 2: Time course of growth, PHA content (a), and composition (b) of the polyester accumulated by R. palustris SP5212 under phototrophic conditions in acetate medium supplemented with valerate as cosubstrate.

The influence of different concentrations of hydroxybutyrate and valerate on growth and polymer synthesis by R. palustris was tested under identical cultural conditions, and the optimum concentration of hydroxybutyrate and valerate for synthesis of PHA was found to be 0.1% (w/v). However, the PHA content differed significantly and was 49.06% and 29.8% CDW for hydroxybutyrate and valerate grown cells respectively. The 3HV monomer unit incorporation was maximum (29.8 mol%) with 0.1% of hydroxybutyrate, while with valerate, the 3HV content increased from 12.56 to 37.6 mol% with increasing concentration (0.05–0.3% w/v) of the cosubstrate used (Table 1). It was evident that the polymer accumulation efficiency and the monomeric composition of the accumulated PHAs by R. palustris SP5212 were correlated with the concentrations of cosubstrate supplemented in the growth medium. Moreover, the strain was able to direct more 3HV monomer (37 mol%) to copolymer with valerate compared to hydroxybutyrate (Table 1). Mutant strain of Rhodobacter sphaeroides U7 when grown in cosubstrate acetate-valerate (40/40 molar ratio) shows the highest accumulation of copolymer (77.42%) with 84.77% fraction of hydroxyvalerate [12].

Table 1: Effect of hydroxybutyrate and valerate on growth and PHA accumulation by R. palustris SP5212.

Concentration, % (w/v)
Growth, g/L
PHA, % CDW
Composition of PHA, Mol%

3HB
3HV

Hydroxybutyrate

    0.05
0.47
23.25
73.70
26.30

    0.10
0.57
49.06
70.19
29.80

    0.20
0.49
36.33
77.18
22.82

    0.30
0.41
16.78
81.98
18.01

Valerate

    0.05
0.52
15.19
87.44
12.56

    0.1
0.50
29.84
85.64
14.36

    0.2
0.44
20.31
71.13
28.87

    0.3
0.39
17.43
62.39
37.61

The isolate was grown in acetate medium supplemented with hydroxybutyrate and valerate as cosubstrate under microaerophilic condition for 12 days at a light intensity of 10,000 lux, total PHA content was estimated according to the method of Ulmer et al. (1994) [18], and growth was determined by biomass dry weight.

The effect of combined supplementation of hydroxybutyrate and valerate in different proportion during the initiation of growth of R. palustris in acetate medium resulted in significant increase in both polymer accumulation and 3HV monomer incorporation in the synthesized PHAs (Table 2). Maximum polymer accumulation (54.0% CDW) was achieved when hydroxybutyrate : valerate ratio was maintained at 3 : 1. The ¹H spectra of this accumulated copolymer showed the incorporation of more than 50 mol% of 3HV monomer unit (Figure 3). Previously, ¹H NMR study was employed to follow the process of accumulation and decomposition of P(3HB) in R. palustris [20]. The ¹H NMR spectral analysis revealed that 3HV monomer content of the polymer was increased further (51 mol%) when mixtures of both alkanoic acids were used at 3 : 1 ratio. The intracellular level of the polymer also rose to more than 54% of CDW (Table 2).

Table 2: Effect of cosupplementation of hydroxybutyrate and valerate on growth and PHA accumulation by R. palustris SP5212.

Hydroxybuty-rate : Valerate
Growth, g/L
PHA,

% CDW
Composition of PHA, Mol%

3HB
3HV

1 : 3
0.49
26.77
57.66
42.33

1 : 1
0.52
46.26
66.61
33.38

3 : 1
0.66
54.71
48.47
51.52

The isolate was grown in acetate medium supplemented with hydroxybutyrate and valerate in different proportion, and other conditions are the same as mentioned under Table 1.

Figure 3: ¹H NMR spectra of polymer extracted from R. palustris SP5212 cells grown under phototrophic conditions in acetate medium supplemented with mixtures of hydroxybutyrate : valerate (3 : 1).

Finally, attempts were made to grow R. palustris SP5212 in biphasic cultivation condition. The organism was initially grown in malate medium for 4 days under phototrophic, microaerobic conditions; cells were harvested aseptically by centrifugation (12,000 ×g), washed in sterile saline solution, and immediately transferred to acetate medium supplemented with either hydroxybutyrate or valerate as cosubstrate. A significant increase in polymer accumulation was recorded under both conditions (Table 3). The PHA content attained 54% and 37% of cell dry weight when grown with hydroxybutyrate and valerate, respectively. Compositional analysis revealed that PHAs derived from hydroxybutyrate and valerate were copolymers of 66% 3HB-co-34% 3HV and 69% 3HB-co-31% 3HV, respectively. These results corroborate the findings of Vincenzini et al. [16], who also recommended two-step cultivation for improved polyester accumulation in R. palustris. Increase in polymer content from 3% to 18% of CDW was achieved when biphasic process was imposed in this particular strain. Rhodobacter sphaeroides 14F showed 3.5 g/L PHA with 60% PHA content when grown in two-stage aerobic dark cultivation at 37–C [10].

Table 3: Biphasic growth and PHA accumulation by R. palustris SP5212 with hydroxybutyrate and valerate as cosubstrate.

Cosubstrate
Incubation, days
Growth, g/L
PHA, % CDW
Composition of PHA, Mol%

3HB
3HV

6
0.42
11.26
72.57
27.42

8
0.50
29.13
68.67
31.32

Hydroxybutyrate
10
0.61
54.17
66.59
33.41

12
0.49
39.47
65.07
34.92

14
0.45
37.34
57.17
42.82

6
0.33
14.22
76.15
23.84

8
0.38
23.20
74.05
25.94

Valerate
10
0.45
37.40
69.13
30.86

12
0.51
29.16
67.03
32.96

14
0.49
25.16
63.96
36.03

The isolate was grown first in malate medium for 4 days, and cells were harvested, washed, and aseptically transferred to acetate media supplemented with 0.1% hydroxybutyrate and 0.1% valerate; other conditions are the same as under Table 1.

4. Conclusion

The potential of R. palustris SP5212 to produce poly(3-hydroxybutyrate-co-3-hydroxyvalerate) under phototrophic microaerophilic conditions has been assessed in acetate medium supplemented with alkanoic acids as cosubstrates. Cosupplementation of mixtures of hydroxybutyrate and valerate as well as biphasic cultivation conditions has improved the PHA accumulation efficiency of the strain significantly, which indicates possible utilization of R. palustris SP5212 for large scale production of PHA copolymers with improved material properties.

Acknowledgment

The authors are grateful to the Council of Scientific and Industrial Research (CSIR), New Delhi, India for financial assistance.

References

A. Steinbüchel, “Perspectives for biotechnological production and utilization of biopolymers: metabolic engineering of polyhydroxyalkanoate biosynthesis pathways as a successful example,” Macromolecular Bioscience, vol. 1, no. 1, pp. 1–24, 2001.

C. S. K. Reddy, R. Ghai, R. Rashmi, and V. C. Kalia, “Polyhydroxyalkanoates: an overview,” Bioresource Technology, vol. 87, no. 2, pp. 137–146, 2003.

H. Brandl, E. J. Knee Jr., R. C. Fuller, R. A. Gross, and R. W. Lenz, “Ability of the phototrophic bacterium Rhodospirillum rubrum to produce various poly (β-hydroxyalkanoates): potential sources for biodegradable polyesters,” International Journal of Biological Macromolecules, vol. 11, no. 1, pp. 49–55, 1989.

G.-Q. Chen and Q. Wu, “The application of polyhydroxyalkanoates as tissue engineering materials,” Biomaterials, vol. 26, no. 33, pp. 6565–6578, 2005.

M. N. Satkowski, D. H. Melik, J. P. Autran, P. R. Freen, I. Noda, and L. A. Schechtman, “Physical and processing properties of polyhydroxyalkanoate copolymer,” in PolyestersII. Propertiesand Chemical Synthesis, Y. Doi and A. Steinbuchel, Eds., vol. 3 of Biopolymers, pp. 231–263, Wiley, Weinheim, Germany, 2001.

B. H. A. Rehm, “Polyester synthases: natural catalysts for plastics,” Biochemical Journal, vol. 376, no. 1, pp. 15–33, 2003.

M. Scandola, G. Ceccorulli, M. Pizzoli, and M. Gazzano, “Study of the crystal phase and crystallization rate of bacterial poly(3-hydroxybutyrate-co-3-hydroxyvalerate),” Macromolecules, vol. 25, no. 5, pp. 1405–1410, 1992.

H. Brandl, R. A. Gross, R. W. Lenz, R. Lloyd, and R. C. Fuller, “The accumulation of poly(3-hydroxyalkanoates) in Rhodobacter sphaeroides,” Archives of Microbiology, vol. 155, no. 4, pp. 337–340, 1991.

M. Liebergesell, E. Hustede, A. Timm et al., “Formation of poly(3-hydroxyalkanoates) by phototrophic and chemolithotrophic bacteria,” Archives of Microbiology, vol. 155, no. 5, pp. 415–421, 1991.

C. Lorrungruang, J. Martthong, K. Sasaki, and N. Noparatnaraporn, “Selection of photosynthetic bacterium Rhodobacter sphaeroides 14F for polyhydroxyalkanoate production with two-stage aerobic dark cultivation,” Journal of Bioscience and Bioengineering, vol. 102, no. 2, pp. 128–131, 2006.

K. Sangkharak and P. Prasertsan, “Nutrient optimization for production of polyhydroxybutyrate from halotolerant photosynthetic bacteria cultivated under aerobic-dark condition,” Electronic Journal of Biotechnology, vol. 11, no. 3, 2008.

K. Kemavongse, P. Prasertsan, A. Upaichit, and P. Methacanon, “Effect of co-substrate on production of poly-β-hydroxybutyrate (PHB) and copolymer PHBV from newly identified mutant Rhodobacter sphaeroides U7 cultivated under aerobic-dark condition,” Songklanakarin Journal of Science and Technology, vol. 29, no. 4, pp. 1101–1112, 2007.

P. Carlozzi and A. Sacchi, “Biomass production and studies on Rhodopseudomonas palustris grown in an outdoor, temperature controlled, underwater tubular photobioreactor,” Journal of Biotechnology, vol. 88, no. 3, pp. 239–249, 2001.

M. Mukhopadhyay, A. Patra, and A. K. Paul, “Production of poly(3-hydroxybutyrate) and poly(3-hydroxybutyrate-co-3- hydroxyvalerate) by Rhodopseudomonas palustris SP5212,” World Journal of Microbiology and Biotechnology, vol. 21, no. 5, pp. 765–769, 2005.

R. De Philippis, A. Ena, M. Guastini, C. Sili, and M. Vincenzini, “Factors affecting poly-β-hydroxybutyrate accumulation in cyanobacteria and in purple non-sulfur bacteria,” FEMS Microbiology Reviews, vol. 103, no. 2-4, pp. 187–194, 1992.

M. Vincenzini, A. Marchini, A. Ena, and R. De Philippis, “H₂ and poly-β-hydroxybutyrate, two alternative chemicals from purple non sulfur bacteria,” Biotechnology Letters, vol. 19, no. 8, pp. 759–762, 1997.

S. Sawayama, K. Tsukahara, T. Yagishita, and S. Hanada, “Characterization of lighted upflow anaerobic sludge blanket (LUASB) method under sulfate-rich conditions,” Journal of Bioscience and Bioengineering, vol. 91, no. 2, pp. 195–201, 2001.

H. W. Ulmer, R. A. Gross, M. Posada, P. Weisbach, R. C. Fuller, and R. W. Lenz, “Bacterial production of poly(β-hydroxyalkanoates) containing unsaturated repeating units by Rhodospirillum rubrum,” Macromolecules, vol. 27, no. 7, pp. 1675–1679, 1994.

B. A. Ramsay, K. Lomaliza, C. Chavarie, B. Dube, P. Bataille, and J. A. Ramsay, “Production of poly(β-hydroxybutyric-co-β-hydroxyvaleric) acids,” Applied and Environmental Microbiology, vol. 56, no. 7, pp. 2093–2098, 1990.

Y. Imai, S. Morita, and Y. Arata, “Proton correlation NMR studies of metabolism in Rhodopseudomonas palustris,” Journal of Biochemistry, vol. 96, no. 3, pp. 691–699, 1984.